# 3M Advanced Materials Division Making products lighter ... Glass...Â Â· Making products lighter. Stronger. Smarter. ... American Coatings Conference 2016 ... Heat reflective roof coatings ...

• Published on
03-Feb-2018

• View
213

0

Embed Size (px)

Transcript

April 12, 2016

Making products lighter. Stronger. Smarter. Better.

• American Coatings Conference 2016

Evaluation of 3M Glass Bubbles for Solar Heat Reflection in Waterborne Acrylic Elastomeric Roof Coatings

Kevin Rink, Senior Technical Service Chemist

Andrea Charif, Applications Development Engineer

3M (St. Paul, MN)

Outline

1. Introduction

2. Definitions

3. Characteristics of Elastomeric

Roof Coatings

4. Materials

5. Formulation & Sample Preparation

6. Testing & Results

Basic Paint

PVC Study

Glass Bubbles compared to commercial

microsphere blend as post addition to

commercial paint

Energy Calculator

7. Summary

Introduction

1. Increase in construction builds = increased energy

demand = higher cooling costs in warmer climates

2. Heat reflective roof coatings (typically white/lighter

colors) are one option used to combat these costs

due to their high solar reflectance and emittance

values in the thermal infrared region.

3. Solar radiation spectrum divided into 3 bands:

UV: 200400 nm 5% of sunlight energy

Visible: 400700 nm 46% of sunlight energy

Near Infrared: 7002500 nm 49% of sunlight energy

felt as heat

Accounts for 96% of radiation in sunlight

Higher SRIs

= higher cumulative solar reflectance

= cooler surfaces

Typical cool roof coatings have TSRs >80%, primarily in visible and infrared regions. (TSR) is a weighted average of solar reflectance at each solar energy wavelength.

Amount of heat radiated per unit area at a given temperature (ability to give up heat).

A combined value of Reflectance and Emittance.*

Standard black surface = 0 (R=5, E=90)

Standard white = 100(R=80, E=90)

Definitions

Solar Reflection

Thermal Emittance

Solar Reflectance Index (SRI)

*Calculations allow for SRIs >100.

These will be evaluated in addition

to thermal effects as related to the

inside temperature.

Elastomeric Roof Coatings: Typical Characteristics

Adhesion (Dry & Wet) to many construction substrates

including polyurethane foams, metal(s), concrete, etc.

Elasticity

Low temperature flexibility & excellent elongation

Water resistance

Low toxicity and easy clean-up

Solar reflectance

UV resistance

DPUR (dirt pick-up resistance)

3M Glass Bubbles

Hollow Glass Microspheres

water resistant soda-lime-borosilicate glass.

3M Glass Bubbles

Appearance White Powder

Crush Strength, psi(90% survival)

25028,000

True Densityg/cc

0.150.6

Median Particle Sizemicrons

1665

Effective Top Particle Size, microns

27120

ProductTarget Crush Strength, psi(90% survival)

True Density(g/cc)

Particle Size Distribution (microns by volume)

10% 50% 90%

Calcium Carbonate (CaCO3)

Hardness: 34 mohs

2.72 -Average =12 microns

-

Glass Bubble 3 (GB3) 16,000 0.46 12 20 30

Glass Bubble 1 (GB1) 250 0.125 30 65 115

Commercial Microsphere Blend (CMB)

(solid particles)

7,000(>98%)

0.73 -Average =

100 microns-

Glass Bubble 2 (GB2) 400 0.22 20 35 65

Commercial W/B Elastomeric Paint

N/A N/A N/A N/A N/A

Materials

Formulations CaCO3(control)

GB3 GB1 CMB GB2

Material WPG Amount (gal) Amount (gal) Amount (gal) Amount (gal) Amount (gal)

Water 8.34 18.23 18.23 18.23 18.23 18.23

Dispersant 10.00 0.50 0.50 0.50 0.50 0.50

Potassium Tripolyphosphate 21.15 0.07 0.07 0.07 0.07 0.07

Cellulosic Thickener 11.61 0.30 0.30 0.30 0.30 0.30

Defoamer 7.10 0.28 0.28 0.28 0.28 0.28

Microbicide 8.33 0.18 0.18 0.18 0.18 0.18

Wetting Agent 8.97 0.22 0.22 0.22 0.22 0.22

Titanium Dioxide 32.33 2.32 2.32 2.32 2.32 2.32

Zinc Oxide 46.82 0.96 0.96 0.96 0.96 0.96

Calcium Carbonate 22.70 18.72 0 0 0 0

100% Acrylic Elastomeric Binder 8.70 54.60 54.60 54.60 54.60 54.60

Defoamer 7.10 0.21 0.21 0.21 0.21 0.21

Coalescent (e.g. Texanol) 7.91 0.76 0.76 0.76 0.76 0.76

Mildewcide 8.60 0.28 0.28 0.28 0.28 0.28

Ammonia (28%) 7.69 0.13 0.13 0.13 0.13 0.13

GB3 3.84 0 18.72 0 0 0

GB1 1.04 0 0 18.72 0 0

Commercial Microsphere Blend 6.1 0 0 0 18.72 0

GB2 1.84 0 0 0 0 18.72

Propylene Glycol 8.66 1.62 1.62 1.62 1.62 1.62

Water 8.34 0.61 0.61 0.61 0.61 0.61

TOTALS 99.99 99.99 99.99 99.99 99.99

Formulations

Adjust viscosity with HASE (Hydrophobically-modified Alkali

Swellable Emulsion) or appropriate thickener to 100-125 KUs

PVC = 42 (details on following slide)

NV (vol) = 52

VOC =

Formulation42 PVC Paint

Raw Material V% Wet V% Dry

TiO2 2.3 5.3

GB, CaCO3 or CMB 18.7 35.3

Acrylic Binder 54.6 56.7

Other Ingredients 24.4 2.7

Sample Preparation

1. Application: Used drawdown bars

and/or cast film(s) on black/white

Leneta charts & 3003 H14 aluminum.

2. Cure: Air dry minimum 72 hours before

testing. QUV samples aged minimum

of 1 week before testing.

Calcium Carbonate Glass Bubble 1 Glass Bubble 2

100 um

Glass Bubble 3Commercial

Microsphere Blend Commercial Paint

Smallest & strongest bubble

Scanning Electron Microscopy (SEM) of finished paint surface: 500X

Images display surface topography of dried film

Test Methods

Property Test Method

Opacity ASTM D2805

Reflectance ASTM E1347, ColorFlex EZ Instrument

Gloss ASTM D523

Dry Film Thickness PosiTector 6000

Solar Reflectance ASTM E903/G173

Solar Reflectance Index Computer model based on ASTM E1980

Thermal Emittance ASTM C1371 (Total Hemispherical at ambient temp 7278F)

Infrared Lamp Test 3M Test Method

QUV Weathering 1000 hours, Proprietary Method (Reference G154)

DPUR Dirt Pick-Up Resistance (24 hours/070 micron Arizona test dust)

• s

Basic Paint Results

Similar gloss and opacities, but Glass Bubbles yield brighter/whiter appearance.

Filler Opacity Reflectance Value Y 60 gloss

GB3 99.5 95.6 5

GB1 99.2 94.9 4.4

GB2 100.0 94.8 4

CaCO3 99.5 92.7 4.5

Commercial Paint 100.3 89.1 3.1

Commercial Microsphere Blend 100.6 87.7 3.5

General Test Results: 1520 mil films

Solar Reflectance

Perkin Elmer Lambda 950 Spectrometer Near IR attachment (scan 2502500 nm)

Solar Reflectance: Aluminum

In general, Glass Bubbles offer very good overall Total Solar Reflectance (TSR).

12.6

12.8

13.0

13.2

13.4

13.6

13.8

70.0

75.0

80.0

85.0

90.0

95.0

100.0

CaCO3 GB3 GB1 commercialmicrosphere

blend

GB2 Commercial Paint

% Reflectance Total Solar Reflectance on 3003 Aluminum

TSR % TSR Visible% TSR IR% TSR UV%

sig

ma

= 0

.5

Solar Reflectance: White Paper

12.4

12.6

12.8

13

13.2

13.4

13.6

13.8

70

75

80

85

90

95

100

CaCO3 GB3 GB1 commercialmicrosphere

blend

GB2 Commercial Paint

% ReflectanceTotal Solar Reflectance on white paper

TSR % TSR Visible% TSR IR% TSR UV%

TSR UV%

Solar Reflectance: Black Paper

12.6

12.7

12.8

12.9

13

13.1

13.2

13.3

13.4

13.5

13.6

60

65

70

75

80

85

90

95

100

CaCO3 GB3 GB1 commercialmicrosphere

blend

GB2 CommercialPaint

% Reflectance Total Solar Reflectance on Black paper

TSR % TSR Visible% TSR IR% TSR UV%

Total Solar Reflectance

Trend is similar on all substrates: Glass Bubbles offer excellent overall TSR.

GB3 (smallest tested) exhibited best solar reflectance at all wavelengths.

60

65

70

75

80

85

90

95

100

nm

31

03

75

44

05

05

57

06

35

70

07

65

83

08

95

960

102

5109

0115

5122

0128

5135

0141

5148

0154

5161

0167

5174

0180

5187

0193

5200

0206

5213

0219

5226

0232

5239

0245

5

Refl

ecta

nce%

Wavelength(nm)

Reflectance on aluminum CaCO3

GB3

GB1

commercialmicrosphere blend

GB2

commercial paint

Black chip calibrated: 0.88

Stainless steel chip calibrated: 0.05

Thermal EmittancePortable unit, total hemispherical emittance

88

89

90

91

92

93

94

95

CaCO3 GB3 GB1 commercialmicrosphere

blend

GB2 commercial paint

% E

mis

siv

ity

Samples

Emissivity %

Emissivity Results

No appreciable differences in emissivity: all samples >90% on aluminum

*Tool coded by Ronnen Levinson, Heat Island Group, Lawrence Berkeley National Laboratory (http://HeatIsland.LBL.gov)

For assistance, contact Hashem Akbari@H_Akbari@LBL.gov, or Ronnen Levinson at RMLLevinson@LBL.gov

Solar Reflectance Index (SRI)Combined calculated value using solar reflectance and emittance (can be >100).

Higher value indicates higher overall reflectance.

SampleThermal

EmittanceTotal Solar

ReflectanceSolar Reflectance

Index (SRI)*Calculated Roof

Surface Temp. (C)

CaCO3 0.93 0.856 108 41.4

GB3 0.92 0.887 113 39.8

GB1 0.92 0.887 113 39.8

Commercial Microsphere Blend

0.93 0.811 102 43.8

GB2 0.91 0.873 111 40.6

Commercial Paint 0.93 0.823 104 43.2

http://heatisland.lbl.gov/mailto:Akbari@H_Akbari@LBL.govmailto:RMLLevinson@LBL.gov

Infrared Lamp Test

IR lamp: Incandescent heat Lamp Light Bulb/

250W/R40 reflector/120V

Red triangle bulbs-T20931 250R40/red

Sample Size: Approx. 6 x 5 cm. (aluminum chip)

Thermocouple: Omega Engineering Type K

with MicroDAQ EL-USB-TC logger

Chip placed on ceramic plate- thermocouple

attached to back side of aluminum through hole

Distance to target: Approx. 10 cm.

Demonstrate effect of filler in coating on inside temperature of buildings

10 cm

Infrared Lamp Test Results

100

110

120

130

140

150

160

170

180

0 20 40 60 80

Te

mp

Pro

file

(

F)

Time (Min)

IR Lamp test -Thermal Insulative Comparison

CaCO3

GB3

GB1

commercialmicrosphere blend

GB2

(Commercial Paint)

Infrared Lamp Test Results

GBs could yield cooler inside temp as simulation shows on back side of aluminum panel.

SampleOverall Avg.

Temperature (F)Avg. After

40 min. (F) from

CaCO3

CaCO3 154.4 167.9 Reference

GB3 145.6 158.3 9.6

GB1 149.6 161 6.9

Commercial Microsphere Blend

155.6 168.3 0.4

GB2 150.5 161.3 6.6

Commercial Paint 161.9 175.9 8.0

• s

PVC Study with Glass Bubble 3

Solar Reflectance: Aluminum

PVC=28 PVC=42 PVC=55

12.8

12.9

13

13.1

13.2

13.3

13.4

70

75

80

85

90

95

100

GB3 9.3vol% GB3 18.7 vol% GB3 29.4 vol%

TSR % TSR Visible% TSR IR% TSR UV%

SRI: Solar Reflectance Index

No significant differences in calculated SRI even at lower loading of GB3.

Sample V% wet V% DryPaint PVC

Thermal Emittance

Total Solar Reflectance

Solar Reflectance Index (SRI)

GB3 9.3 20 28 0.93 0.879 112

GB3 18.7 35 42 0.93 0.887 113

GB3 29.4 50 55 0.92 0.883 112

SampleOverall

Avg. Temp (F)

Avg. After

40 Min.

(F) From

CaCO3

CaCO318.7%

154.4 167.9 Reference

GB3 9.3% 148.2 161 6.9

GB3 18.7% 145.6 158.3 9.6

GB3 29.4% 141.7 153.5 14.4

Infrared Lamp Test Results

75

95

115

135

155

175

0 20 40 60 80

Tem

p P

rofi

le

(F)

Time (min)

IR Lamp Test GB 3

GB3(9.3% vol)

GB3(18.7% vol)

GB3(29.4% vol)

Accelerated Weathering: 1000 Hours QUV

Glass bubbles exhibited good gloss retention, and comparable color retention and DPUR.

3 mil dry film thickness

Sample% 60

Gloss LossTotal Color

Change (DE)

DPUR(% Reflectance Recovery After

QUV and 24 Hour Dry Dirt Test)

CaCO3 38 0.4 96.2

GB3 0 0.27 97.0

GB1 0 0.45 94.5

Commercial Microsphere Blend

4 0.42 96.2

GB2 0 0.37 95.2

Commercial Paint 19 1.57 95.5

• s

Glass Bubble 3 vs.Commercial Microsphere Blend

Total Solar Reflectance

Post Addition of GB3 to commercial paint also increased total solar reflectance.

GB3 vs. Commercial Microsphere Blend

55

60

65

70

75

80

85

90

95

25

0

34

0

43

0

52

0

610

70

0

79

0

88

0

97

0

106

0

115

0

124

0

133

0

142

0

1510

160

0

169

0

178

0

187

0

196

0

20

50

214

0

22

30

23

20

24

10

25

00

% R

efl

ec

tan

ce

Wavelength(nm)

Commercialpaint+GB3

CommercialPaint+commercialmicrosphere blend

IR Lamp Test

Post addition of glass bubbles could yield cooler inside temp as simulation

shows on back side of aluminum panel.

Comparing GB3 vs Commercial Microsphere Blend

Energy Cost Calculators: \$\$

Input in = Input out

One example: http://web.ornl.gov/sci/roofs+walls/facts/CoolCalcEnergy.htm

TSR EmittanceEnergy Cost

(\$/kwH)

*Savings Over Black Roof (\$/ft2/year)

CaCO3 85.6 93 0.2 0.407GB3 88.7 92 0.2 0.421GB1 88.7 92 0.2 0.421

Commercial Microsphere Blend 81.1 93 0.2 0.384GB2 87.3 91 0.2 0.412

Commercial Paint 82.3 93 0.2 0.391

*R value PlaceAir Conditioner

EfficiencyHeat

Heat Cost (\$/kwH)

Heat Efficiency

10 Miami, FL 2 Electric 0.2 0.7

Many factors can affect overall savings calculations

http://web.ornl.gov/sci/roofs+walls/facts/CoolCalcEnergy.htm

Summary

Smaller glass bubbles (GB3) may offer other benefits such as performance in darker colors and

TSR after extended outdoor exposure.

Property Benefits of 3M Glass Bubbles

Total Solar Reflectance

Total Emissivity Insulative Properties/Lower

Inside Temperature

Energy Savings

*Weatherability/DPUR

Further optimization

work is recommended

to quantify other

benefits such as

benefits in darker

colors & TSR after

outdoor exposure.

Acknowledgements

Andrea Charif, Applications Development Engineer (3M St. Paul)

Jean-Marie Ruckebusch, Senior Technical Service Specialist (3M France)

Connie Forehand, Laboratory Technician (3M St. Paul)

Andy Peterson, Laboratory Technician (3M St. Paul)

Terri Shefelbine, Senior Product Development Chemist (3M St. Paul)

Warranty, Limited Remedy, and Disclaimer: Many factors beyond 3Ms control and uniquely within users knowledge and

control can affect the use and performance of a 3M product in a particular application. User is solely responsible for evaluating

the 3M product and determining whether it is fit for a particular purpose and suitable for users method of application. User is

solely responsible for evaluating third party intellectual property rights and for ensuring that users use of 3M product does not

violate any third party intellectual property rights. Unless a different warranty is specifically stated in the applicable product

literature or packaging insert, 3M warrants that each 3M product meets the applicable 3M product specification at the time

3M ships the product. 3M MAKES NO OTHER WARRANTIES OR CONDITIONS, EXPRESS OR IMPLIED, INCLUDING, BUT

NOT LIMITED TO, ANY IMPLIED WARRANTY OR CONDITION OF MERCHANTABILITY OR FITNESS FOR A PARTICULAR

PURPOSE OR ANY IMPLIED WARRANTY OF NON-INFRINGEMENT OR ANY IMPLIED WARRANTY OR CONDITION

ARISING OUT OF A COURSE OF DEALING, CUSTOM OR USAGE OF TRAD...